Access the full text.

Sign up today, get DeepDyve free for 14 days.

SPIE Reviews
, Volume 1 (1) – Jan 1, 2010

/lp/spie/negatively-refracting-chiral-metamaterials-a-review-7YaQjUyo0y

- Publisher
- SPIE
- Copyright
- Copyright © 2011 COPYRIGHT SPIE--The International Society for Optical Engineering. Downloading of the abstract is permitted for personal use only.
- ISSN
- 1946-3251
- DOI
- 10.1117/6.0000003
- Publisher site
- See Article on Publisher Site

Abstract. Chirality extends the class of negatively refracting metamaterials by endowing a richer palette of electromagnetic properties. Chiral metamaterials can support negative refraction, which must be assessed in light of the closely related phenomenons of negative phase velocity and counterposition. Two categories of chiral metamaterials are being examined these days: (a) homogeneous and homogenizable chiral materials, as exemplified by isotropic chiral materials, Faraday chiral materials, and materials with simultaneous mirror-conjugated and racemic chirality characteristics; and (b) structurally chiral materials, as exemplified by helicoidal bianisotropic materials and ambichiral materials. The planewave response of a half-space occupied by a chiral metamaterial is complex, and important distinctions between negative refraction, negative phase velocity, and counterposition emerge. C 2010 Society of Photo-Optical Instrumentation Engineers. [DOI: 10.1117/6.0000003] Keywords: negative phase velocity; ambichirality; Faraday chiral material; mirror conjugation; racemic chirality; counterposition; helicoidal bianisotropic materials; negative refraction. Paper SR090107 received Jul. 21, 2009; revised manuscript received Sep. 19, 2009; accepted for publication Sep. 19, 2009; published online Jan. 14, 2010. 1 Introduction Probably the first engineered composite materials were bronze alloys made by smelting copper and tin together more than 5000 years ago. Research on mechanical properties of composite materials has a very rich history, the earliest parts of which are shrouded in the mists of time. Glass too was perhaps created in the Bronze Age, and colored glasses fabricated by mixing some particulate material in silica date back to more than two millenniums ago. Systematic research on optical properties of composite materials began two centuries back, with the publication of the Arago-Biot formula [1]. Since then, theoretical and experimental research continues unabated [2â€“5]. A composite material must have at least two constituent materials. Each constituent material is chemically inert with respect to the others in its immediate proximity within the composite material. This restriction excludes molecularly pure materials containing two or more types of atoms from being classified as composite materials. Metamaterials are also composite materials, but with a difference. A metamaterial exhibits response characteristics that either (i) are not observed in or (ii) are enhanced relative to the individual responses of its constituent materials [6]. This characterization of metamaterials captures the notion originally proposed by Walser who envisaged them as being artificial materials fabricated by first downscaling macroscopic material architectures to the submicron and the nanometer length scales and then combining different downscaled architectures into macroscopic materials that would exceed their conventional counterparts in performance [7]. Possessing a cellular morphology, nanoengineered metamaterials may satisfy 1946-3251/2010/$25.00 SPIE Reviews 2010 SPIE 018003-1 Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . Fig. 1 Left-handed and right-handed enantiomers of a generic amino acid. (Courtesy of NASA.) complex multifunctional requirements by a judicious juxtaposition of sufficiently small cells of different materials, shapes, and sizes [8]. Our focus in this review is on negatively refracting metamaterials. Millions of research dollars have been spent during the last decade on this topic, following experimental reports of negative refraction in certain metamaterials under microwave illumination [9,10]. Research activity has been greatly fuelled by the possibility of fabricating planar lenses with very high resolving power [11]. Within the past couple of years, metamaterials that exhibit negative refraction at optical frequencies have been developed [12â€“15], and current efforts are directed toward reducing the considerable dissipative losses associated with optical negative refraction [16,17]. Parenthetically, we note that negative refraction is not exclusive to artificial metamaterials: certain biological structures [18] and naturally occurring minerals [19] also exhibit negative refraction. The simplest materials that exhibit negative refraction are isotropic dielectric-magnetic materials [20], but the scope for exotic behavior such as negative refraction is considerably increased if chirality is introduced [21â€“24], especially in combination with anisotropy [25,26] or nonhomogeneity [27,28]. We confine ourselves in this review to chiral and certain related metamaterialsâ€”that too of the linear, passive kind. An object is said to be chiral if it cannot be made to coincide with its mirror image by translations and/or rotations. A remarkable property of chiral materials is that they can discriminate between left-handed and right-handed electromagnetic waves [29]. In order to achieve this discrimination, handedness is necessarily intrinsic to chiral materials. Handedness is manifest in the microstructure of homogeneous and homogenizable chiral materials. For example, an isotropic chiral material comprises a random dispersion of handed molecules or inclusions [29]. An illustration of handed molecules is provided in Fig. 1. In contrast, handedness is manifest at the macroscopic level in structurally chiral materials. For example, the molecules of cholesteric liquid crystals are randomly positioned but macroscopically they exhibit a helicoidal orientational order [30,31], as represented in Fig. 2. Other examples of structurally chiral materials can be fabricated either as stacks of uniaxial laminas [32] or using thin-film technology [33]. Remarkably, artificial examples of both types of chiral materials were produced by Bose more than 11 decades ago [34]. Parenthetically, a third type of â€œchiralâ€ medium has recently entered scientific literature [35,36]. Such a material is made by depositing spirals (and similar objects) on some flat surface. Spirals, being essentially two-dimensional objects, cannot be chiral, and â€œplanar chiralityâ€ [37,38] is an infelicitous term that ought to be replaced by a meaningful term. SPIE Reviews 018003-2 Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . Fig. 2 A representation of a cholesteric liquid crystal (also known as a chiral nematic liquid crystal) that is structurally chiral. Adjacent liquid crystal molecules are twisted relative to their neighbors. (Courtesy of Kevin G. Yager, National Institute of Standards and Technology, Gaithersburg, MD, USA.) In the following sections, we highlight the propensity of chiral metamaterialsâ€”of the homogeneous and homogenizable type and of the structurally chiral typeâ€”to exhibit negative refraction. Let us remark that, in addition to negative refraction, isotropic [39,40] and bianisotropic [41] chiral materials can support the allied phenomenon of negative reflection under certain conditions. As regards notational matters: vectors are denoted by boldface with unit vectors being identified by an additional caret. Sans serif boldface indicates either a 3Ã—3 dyadic or a 4Ã—4 matrix, and the 3Ã—3 identity dyadic is written as I. The real and imaginary parts of complexvalued quantities are written as Re (Â·) and Im(Â·); the superscript âˆ— denotes the complex conjugate; âˆš and i = âˆ’1. The permittivity and permeability of free space (i.e., vacuum) are written as 0 âˆš and Î¼0 , respectively, and c0 = 1/ 0 Î¼0 . An exp(âˆ’iÏ‰t) dependence on time is implicit, where Ï‰ is the angular frequency and t is time. 2 Homogeneous and Homogenizable Chiral Materials 2.1 Preliminaries The characterization of negative refraction by chiral materials is considerably more complicated than of negative refraction by isotropic dielectric-magnetic materials, as more than one refraction wavevector needs to be considered as well as magnetoelectric coupling and possibly directionality [42]. Negative phase velocity (NPV) has been widely adopted as a convenient indicator of negative refraction [43,44]. While NPV and negative refraction go hand-in-hand for uniform planewave propagation in isotropic dielectric-magnetic materials, this is not generally true for nonuniform plane waves, especially in anisotropic materials. The possibility of NPV SPIE Reviews 018003-3 Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . propagation in chiral materials was evident some years ago [45], but only nowadays is it being considered carefully [46â€“54]. Distinctions that can arise between negative refraction and NPV, as well as the closely related phenomenon of counterposition, in chiral metamaterials are highlighted in Sec. 2.5. Here we consider NPV propagation of uniform plane waves in certain well-known chiral materials and metamaterials.âˆ— Let us consider electromagnetic field phasors Ë† E(r) = E0 exp(ik k â€¢ r) Ë† H(r) = H0 exp(ik k â€¢ r) , (1) Ë† Ë† with complex-valued wavenumber k and wavevector k = k k (|k| = 1), in various types of homogeneous (or homogenizable) chiral materials. These materials are all included in the most general linear category of materials, namely bianisotropic materials, which are characterized by the frequency-domain constitutive relations [55] D(r) = â€¢ E(r) + Î¾ â€¢ H(r) . (2) B(r) = Î¶ â€¢ E(r) + Î¼ â€¢ H(r) Combining Eqs. (1) and (2) with the source-free Maxwell curl postulates leads to the algebraic equation L(k) â€¢ E(r) = 0, where the 3Ã—3 dyadic L(k) = (k Ã— I + Ï‰Î¾ ) â€¢ Î¼âˆ’1 â€¢ (k Ã— I âˆ’ Ï‰Î¶ ) + Ï‰2 . Solution of the dispersion relation det [ L(k) ] = 0 (5) (4) (3) delivers the permissible wavenumbers. Since Eq. (5) represents a quartic polynomial, there are generally four wavenumbers, but the symmetries of the constitutive dyadics , Î¾, Î¶ and Î¼ may result in the number of independent wavenumbers being less than four. The phase velocity of the plane wave is classified as negative or positive, depending upon whether the scalar product Re ( k) â€¢ P(r) is negative or positive, where P(r) = 1 Re [E(r) Ã— Hâˆ— (r) ] 2 (6) is the time-averaged Poynting vector. As discussed in Sec. 2.5, the phase velocity can also be orthogonal to the time-averaged Poynting vector; i.e., Re (k) â€¢ P(r) = 0. The ratio of k to k0 = Ï‰/c0 may be called a refractive index. 2.2 Isotropic Chiral Materials The simplest chiral materials to consider are the isotropic chiral materials (ICMs). An everyday example of a homogeneous ICM is represented by an aqueous solution of dextrose at optical frequencies [56,57]. As another example, consider a random assembly of right-handed springs, each âˆ¼2 mm long and âˆ¼1 mm in diameter. While this assembly is nonhomogeneous at optical frequencies, it represents a homogenizable chiral material whose chirality is manifest under âˆ— In Sec. 2.5 both uniform and nonuniform plane waves are considered. 018003-4 Vol. 1, 2010 SPIE Reviews Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . Fig. 3 An isotropic chiral material fabricated for microwave applications. Miniature springs are Â´ randomly dispersed in epoxy. (Courtesy of Alvaro Gomez, Universidad de Cantabria, Spain.) Â´ microwave illumination [58â€“60]. Notice that the latter example represents a chiral metamaterial whereas the former does not. An illustration of an ICM fabricated for microwave applications is provided in Fig. 3. Mathematically, ICMs are described by their frequency-domain constitutive relations [29] D(r) = E(r) + iÎ¾ H(r) B(r) = âˆ’iÎ¾ E(r) + Î¼H(r) (7) where Î¾ is the chirality parameter. Equation (5) delivers four possible wavenumbers, k = (1) (2) (3) (4) kI CM , kI CM , kI CM , and kI CM , where âˆš (1) Î¼+Î¾ kI CM = âˆ’Ï‰ âˆš (2) kI CM = Ï‰ Î¼âˆ’Î¾ kI CM = âˆ’kI CM kI CM = âˆ’kI CM SPIE Reviews 018003-5 (4) (1) (3) (2) âŽ« âŽª âŽª âŽª âŽª âŽª âŽª âŽ¬ âŽª âŽª âŽª âŽª âŽª âŽª âŽ . (8) Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . If the inequalities âŽ› Re âˆš Î¼ + Î¾ Ã— Re âŽ âŽ› Re âˆš Î¼ âˆ’ Î¾ Ã— Re âŽ âˆ— âŽž âŽ <0 âŽž âŽ <0 for for k= Î¼âˆ— âˆ— âŽª (1),(4) âŽª kI CM âŽª âŽª âŽª âŽª âŽ¬ (9) âŽ« âŽª Î¼âˆ— âŽª âŽª âŽª (2),(3) âŽª k = kI CM âŽª âŽª âŽª âŽ are satisfied, then NPV propagation is supported [24]. For a nondissipative isotropic chiral (1),(2),(3),(4) material (i.e., , Î¾, Î¼ âˆˆ R) with kI CM âˆˆ R, the NPV conditions [Eqs. (9)] reduce to âˆš âˆš Î¼ < âˆ’Î¾ Î¼<Î¾ for for k = kI CM k = kI CM (2),(3) (1),(4) (10) Thus, we observe that NPV propagation arises only when the magnitude of the chirality âˆš Î¼ [24,61]. Furthermore, the parameter Î¾ is sufficiently large relative to the magnitude of (1),(4) phase velocity can be positive for the plane waves with wavenumbers kI CM but negative for (2),(3) the plane waves with wavenumbers kI CM , or vice versa [62]. The boundary between positive and negative phase velocity is characterized by infinite phase velocity [63]. The NPV conditions in Eqs. (9) and (10) highlight a key difference between ICMs and isotropic dielectric-magnetic materials. For the latter (which are described by the constitutive relations in Eq. (7) but with Î¾ = 0), NPV arises when the inequality Re ( ) Re (Î¼) + <0 Im ( ) Im (Î¼) (11) is satisfied [44]. For passive isotropic dielectric-magnetic materials, a sufficient set of conditions for NPV is therefore Re ( ) < 0 and Re (Î¼) < 0. In practice, Re ( ) < 0 may be achieved using metallic materials and Re (Î¼) < 0 may be achieved using a microstructure based on split-ring resonators (SRRs), but it proves to be tricky to satisfy both of these conditions at the same frequency [20]. The introduction of chirality enables NPV to achieved without it being necessary for Eq. (11) (or Re ( ) < 0 and Re (Î¼) < 0) to be met. Furthermore, relatively âˆš Î¼ is close to zero. A strong chiral effects may be realized provided that the magnitude of recent example is represented by the chiral metamaterial developed by Wang et al. [54], which exhibits a negative refractive index in the gigahertz frequency range. As shown in Fig. 4, their metamaterial is constructed from SRRs that are arranged on a cubic Bravais lattice. Theoretical and experimental studies confirm that the real part of the refractive index for one wavenumber is negative-valued, as illustrated in Fig. 5. âˆš The prospects of | Î¼| being close to zero, and thereby satisfying the conditions for NPV, may be enhanced through exploiting materials with either | | â‰ˆ 0 or |Î¼| â‰ˆ 0 [64]. Such â€œepsilonnear-zeroâ€ metamaterials have recently been considered for antenna [65], imaging [66], and tunneling [67] applications, whereas â€œmu-near-zeroâ€ metamaterials have been considered for cloaking applications [68]. The canonical case of â€œepsilon-near-zeroâ€ and â€œmu-near-zeroâ€ for achiral materials is represented by nihility [69], wherein = Î¼ = 0. By restricting the notion of nihility to a particular frequency regime, and incorporating a nonzero chirality parameter Î¾ , the notion of chiral nihility emerges [21]. 2.3 Faraday Chiral Materials Suppose we have a random mixture of (i) an isotropic chiral material [29], as described by the frequency-domain constitutive relations in Eqs. (7), and (ii) either a magnetically biased SPIE Reviews 018003-6 Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . Fig. 4 The chiral metamaterial of Wang et al. [54]. Four split-ring resonators (a) are locked together to form the unit cell (b); and these unit cells are then arranged on a cubic lattice (c). (Reprinted with permission from Ref. 54. Copyright 2009 by the American Institute of Physics.) Simulation 4 n+ 2 0 âˆ’2 4 nâˆ’ 2 0 âˆ’2 n&Îº 2 0 âˆ’2 (e) 6 (c) â„œ(n) â„œ(Îº) (f) (a) â„œ(nâˆ’) â„‘(nâˆ’) (d) â„œ(n) â„œ(Îº) â„œ(n+) â„‘(n+) (b) â„œ(nâˆ’) â„‘(nâˆ’) Experiment â„œ(n+) â„‘(n+) 7 8 9 6 7 8 9 Frequency (GHz) Frequency (GHz) Fig. 5 Theoretical and experimental values of refractive indexes for the chiral metamaterial of âˆš Wang et al. [54] at gigahertz frequencies. Here, Îº = c 0 Î¾ and n = c 0 Î¼, with n Â± = n Â± Îº being the refractive indexes for left- and right-handed waves. According to both theory and experiment, the real part of the index n + is negative at 7.7 GHz. (Reprinted with permission from Ref. 54. Copyright 2009 by the American Institute of Physics.) plasma [70], as described by the frequency-domain constitutive relations D(r) = gyro â€¢ E(r) B(r) = Î¼0 H(r) (12) or a magnetically-biased ferrite [71], as described by the frequency-domain constitutive relations D(r) = E(r) B(r) = Î¼ gyro â€¢ H(r) SPIE Reviews 018003-7 (13) Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . wherein the 3Ã—3 constitutive dyadics have the gyrotropic form Ë†Ë† Ë† Ï„ gyro = Ï„ I âˆ’ iÏ„g u Ã— I + (Ï„u âˆ’ Ï„ ) uu, (Ï„ = , Î¼) . (14) Ë† The unit vector u identifies the direction of the biasing magnetic field. The mixture may be regarded as effectively homogeneous provided that wavelengths are much longer than the nonhomogeneities of the mixture. The resulting homogenized composite material (HCM)â€”which is known as a Faraday chiral materialâ€”combines natural optical activity, as exhibited by the isotropic chiral constituent material, with Faraday rotation, as exhibited by the gyrotropic constituent material [72]. Provided that the constituent materials are envisioned as electrically small spherical particles, the Faraday chiral material is described by the frequency-domain constitutive relations [73] D(r) = H CM â€¢ E(r) + iÎ¾H CM â€¢ H(r) B(r) = âˆ’iÎ¾H CM â€¢ E(r) + Î¼H CM â€¢ H(r) where the three 3Ã—3 constitutive dyadics have the common form H H Ë† Ë†Ë† Ï„H CM = Ï„ H CM I âˆ’ iÏ„g CM u Ã— I + Ï„u CM âˆ’ Ï„ H CM uu, (15) (Ï„ = , Î¾, Î¼) . (16) More general Faraday chiral materials can arise through the homogenization of composite materials comprising nonspherical particles [74,75]. The constitutive properties of such HCMs can be estimated using a homogenization formalism. While many different formalisms have been developed [3], the strong-property-fluctuation theory [76,77] provides the basis for a particularly sophisticated homogenization formalism that has been developed for isotropic [78] and anisotropic [75] chiral HCMs. As well as the requirement that the constituent particles of a composite material be electrically small [79,80], the implementation of homogenization formalisms requires that the particles are numerous and distributed statistically uniformly throughout the composite material. Therefore, claims of negative refraction in a chiral metamaterial based on the homogenization of a composite material containing a single chiral inclusion must be regarded warily [81]. In a similar vein, the notion of homogenization precludes the possibility of the constituent materials containing resonant inclusions. Accordingly, claims of a negatively refracting chiral metamaterial arising from the homogenization of resonant inclusions must be viewed with caution too [82]. At best, one can obtain the constitutive parameters of an equivalent homogeneous medium that can replicate the experimental and/or numerical results obtained for a specific source-scatterer-detector configuration [83], but there is no guarantee that those constitutive parameters would be acceptable if the location of the source, the location of the detector, and/or the shape and size of the scatterer were to change without alteration of the composite material that the scatterer is made of. Planewave propagation in Faraday chiral materials is rather more complicated than it is for isotropic chiral materials, because the effects of directionality come into play. For definiteness, Ë† Ë† let us choose the unit vector u = z and consider propagation in the xz plane; i.e., Ë† Ë† Ë† k = x sin Î¸ + z cos Î¸. Equation (5) then has the form [25] a4 with coefficients a4 = ( sin2 Î¸ + SPIE Reviews (17) k Ï‰ + a3 k Ï‰ + a2 k Ï‰ + a1 k Ï‰ + a0 = 0 , (18) cos2 Î¸ )(Î¼ sin2 Î¸ + Î¼z cos2 Î¸ ) âˆ’ (Î¾ sin2 Î¸ + Î¾z cos2 Î¸ )2 , 018003-8 (19) Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . a3 = 2 cos Î¸ sin2 Î¸ [Î¼g ( Î¾z âˆ’ + 2 cos2 Î¸ Î¾g a2 = sin2 Î¸ Î¼Î¼z 2 g z Î¼z zÎ¾ ) g (Î¼Î¾z âˆ’ Î¼z Î¾ ) + Î¾g (Î¼ + Î¼z âˆ’ 2Î¾ Î¾g )] (20) 2 âˆ’ Î¾z , 2 + Î¾ 2 + Î¾g (Î¼ z z 2 + Î¼z ) âˆ’ 2Î¾ Î¾z Î¾g âˆ’ Î¾ 2 + Î¼g z Î¾g âˆ’ âˆ’ 2 g [Î¾z (Î¼g Î¾ âˆ’ Î¼Î¾g ) + Î¼z Î¾ Î¾g ] âˆ’ + 2 cos2 Î¸ a1 = 4 cos Î¸ a0 = z Î¼z 2 âˆ’ Î¾z z Î¼z 2 2 âˆ’ Î¾z 3Î¾g âˆ’ Î¾ 2 âˆ’ Î¼2 âˆ’ Î¼2 + 2Î¾z (Î¼Î¾ âˆ’ Î¼g Î¾g ) g âˆ’ Î¼ , g Î¼g g Î¼g (21) , g Î¼g ) z Î¼z 2 2 âˆ’ Î¾z Î¾ ( g Î¼ + Î¼g ) + Î¾g Î¾g âˆ’ Î¾ 2 âˆ’ Î¼ âˆ’ (22) âˆ’ 2 g 2 Î¼2 âˆ’ Î¼2 + Î¾g âˆ’ Î¾ 2 g 2 âˆ’ 2 Î¾g + Î¾ 2 ( Î¼ + + 4Î¾ Î¾g ( Î¼g + Î¼ g ) . (1) (2) (3) (4) (23) Hence, four independent wavenumbers k = kF CM , kF CM , kF CM , and kF CM may be extracted as the roots of Eq. (18). Propagation with NPV is supported provided that the real-valued scalar WF CM < 0, where WF CM = Re (k)Re + 1 (Î¼âˆ— )2 âˆ’ 2 Î¼âˆ— g 1 Ëœâˆ— âˆ— k sin Î¸ âˆ’ iÎ¾z Î² âˆ— sin Î¸ Î¼âˆ— z Ëœ k âˆ— Î¼âˆ— (|Î±|2 + 1) + iÎ¼âˆ— (Î± âˆ’ Î± âˆ— ) cos2 Î¸ g + Î¼âˆ— |Î²|2 sin2 Î¸ âˆ’ [Î¼âˆ— (Î± âˆ— Î² + Î±Î² âˆ— ) + iÎ¼âˆ— (Î² âˆ’ Î² âˆ— )] sin Î¸ cos Î¸ g âˆ— + Î¼âˆ— Î¾g âˆ’ Î¼âˆ— Î¾ âˆ— [(|Î±|2 + 1) cos Î¸ âˆ’ Î± âˆ— Î² sin Î¸ ] g âˆ— âˆ’ i Î¼âˆ— Î¾ âˆ— âˆ’ Î¼âˆ— Î¾g [(Î± âˆ’ Î± âˆ— ) cos Î¸ âˆ’ Î² sin Î¸ ] g (24) and Î± and Î² are defined in terms of entries of L(k) per âŽ« [ L ]12 [ L ]33 + [ L ]13 [ L ]23 âŽª âŽª âŽª [ L ]13 [ L ]13 âˆ’ [ L ]11 [ L ]33 âŽ¬ . âŽª [ L ]12 [ L ]23 âˆ’ [ L ]13 [ L ]22 âŽª âŽª Î²= âŽ [ L ]13 [ L ]23 + [ L ]12 [ L ]33 Î±= (25) Matters simplify considerably when propagation is parallel to the z axis (i.e., Î¸ = 0). The four independent wavenumbers then reduce to âŽ« (1) kF CM = Ï‰ + g Î¼ + Î¼g âˆ’ Î¾ âˆ’ Î¾g âŽª âŽª âŽª âŽª âŽª (2) âŽ¬ kF CM = Ï‰ âˆ’ + g Î¼ + Î¼g âˆ’ Î¾ âˆ’ Î¾g âŽª (26) (3) âŽª kF CM = Ï‰ âˆ’ g Î¼ âˆ’ Î¼g + Î¾ âˆ’ Î¾g âŽª âŽª âŽª âŽª âŽª âŽ (4) kF CM = Ï‰ âˆ’ âˆ’ g Î¼ âˆ’ Î¼g + Î¾ âˆ’ Î¾g and the NPV parameter WF CM for each wavenumber becomes WF CM = 2 Re SPIE Reviews Î¼ + Î¼g âˆ’ Î¾ âˆ’ Î¾g Re 018003-9 âˆ— + + Î¼âˆ— âˆ— g Î¼âˆ— g for k = kF CM , (1) (27) Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . Fig. 6 The chiral metamaterial of Zhang et al. [84]. The microstructure comprises inductorcapacitor circuits (a) and (b). These are arranged in a tilted conï¬guration to form the metamaterial (c) and (d). (Reprinted with permission from Ref. 84. Copyright 2009 by the American Physical Society.) WF CM = 2 Re Î¼ + Î¼g + Î¾ + Î¾g Re âˆ— Î¼âˆ— + âˆ— âˆ— g Î¼âˆ— g for k = kF CM , (2) (28) WF CM = 2 Re âˆ’ Î¼ âˆ’ Î¼g + Î¾ âˆ’ Î¾g Re âˆ’ âˆ’ âˆ’ âˆ’ Î¼âˆ— âˆ— âˆ— g Î¼âˆ— g for k = kF CM , (3) (29) WF CM = 2 Re âˆ’ Î¼ âˆ’ Î¼g âˆ’ Î¾ + Î¾g Re Î¼âˆ— âˆ— g Î¼âˆ— g for k = kF CM . (4) (30) Numerical studies on the homogenization of an isotropic chiral material and a magnetically biased ferrite have revealed that the resulting Faraday chiral material can support NPV propagation provided that the gyrotropic constitutive parameter of the ferrite constituent material is sufficiently large in magnitude relative to the corresponding magnitudes of nongyrotropic permeability parameters [25]. In particular, Faraday chiral materials can support NPV propagation when their constituent materials do not. A chiral metamaterial with constitutive relations very similar to those of the Faraday chiral material (15) has been developed recently by Zhang et al. [84]. As represented in Fig. 6, their metamaterial comprises metallic chiral resonators in which the loop of the resonator is tilted with respect to a reference plane. This metamaterial exhibits a negative-real refractive index for one wavenumber at frequencies between 1.06 and 1.27 THz, as shown in Fig. 7, despite the magnetic permeability having a positive real part over this frequency range. SPIE Reviews 018003-10 Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . Fig. 7 Experimental values of refractive indexes (nL for left-handed waves and nR for right-handed waves) for the chiral metamaterial of Zhang et al. [84], plotted against frequency (in terahertz). Also plotted are the dielectric, magnetic, and magnetoelectric constitutive parameters , Î¼, and Î¾ respectively. Real parts are in black and imaginary parts are in gray. The real part of the index nL is negative between 1.06 and 1.27 THz. (Reprinted with permission from Ref. 84. Copyright 2009 by the American Physical Society.) 2.4 Materials with Simultaneous Mirror-Conjugated and Racemic Chirality Characteristics Let us next consider an isotropic chiral material described by the constitutive relations in Eq. (7). The mirror conjugate material is also an isotropic chiral material, described by the constitutive relations in Eq. (7) but with the chirality parameter Î¾ replaced by âˆ’Î¾ . When an isotropic chiral material and its mirror conjugate are mixed together in a random fashion, in equal proportions (and provided that no chemical reactions or molecular conformational changes occur), the resulting racemic mixture is an isotropic dielectric-magnetic material; i.e., it is achiral. However, an isotropic chiral material and its mirror conjugate can be mixed together in equal proportions and yet retain chirality, thereby producing a material with simultaneous mirror-conjugated and racemic chirality (SMCRC) characteristics. This can be achieved by fixing the orientations of the chiral elements that make up the constituents of the mixture. For example, an artificial SMCRC SPIE Reviews 018003-11 Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . material may be conceptualized as a mixture of equal proportions of left-handed springs aligned along the x axis and right-handed springs along the y axis; and left- as well as right-handed springs in equal proportions aligned along the z axis [85]; all springs are electrically small. Also, certain naturally occurring minerals exhibit SMCRC below their NÂ´ el temperatures [86,87]. e The 3Ã—3 constitutive dyadics of an SMCRC material may be expressed as âŽ« Ë†Ë† âŽª xË† Ë† Ë† = 1 (Ë† x + yy) + 3 zz âŽª âŽª âŽª âŽª âŽ¬ Î¾ = Î¾ (Ë† x âˆ’ yy) xË† Ë† Ë† . (31) âŽª Î¶ = âˆ’Î¾ âŽª âŽª âŽª âŽª âŽ Ë†Ë† Î¼ = u1 (Ë† x + yy) + Î¼3 zz xË† Ë† Ë† Equation (5) yields the four wavenumbers k = kSMCRC , kSMCRC , kSMCRC , and kSMCRC . However, since SMCRC materials are Lorentz-reciprocal [88], there are only two independent wavenumbers, at most. For propagation in an arbitrary direction given by Ë† Ë† Ë† Ë† k = x sin Î¸ cos Ï† + y sin Î¸ sin Ï† + z cos Î¸, the wavenumbers are [85] âŽ« (1) kSMCRC = Ï‰ b3 (b1 âˆ’ b2 ) âŽª âŽª âŽª âŽª âŽª âŽª (2) (1) âŽ¬ kSMCRC = âˆ’kSMCRC (3) âŽª kSMCRC = Ï‰ b3 (b1 + b2 ) âŽª âŽª âŽª âŽª âŽª âŽ (4) (3) kSMCRC = âˆ’kSMCRC (1) (2) (3) (4) (32) (33) wherein the scalars b1 = 2 z Î¼z cos2 Î¸ + ( z Î¼ + Î¼z ) sin2 Î¸ b2 = sin2 Î¸ ( z Î¼ âˆ’ Î¼z )2 âˆ’ 4 z Î¼z Î¾ 2 cos2 2Ï† 1 b3 = ( Î¼ + Î¾ 2 ) ( sin2 Î¸ + 2 âŽ« âŽª âŽª âŽª âŽª âŽ¬ âŽª âŽª âŽª âˆ’1 âŽª âŽ (34) cos2 Î¸ )(Î¼ sin2 Î¸ + Î¼z cos2 Î¸ ) + Î¾ 2 sin4 Î¸ cos2 2Ï† are introduced. Propagation of plane waves with NPV is supported provided that the real-valued scalar WSMCRC < 0, where [26] WSMCRC = Re (k) 1 (|Î±|2 + |Î²|2 ) cos2 Î¸ + sin2 Î¸ Ï‰ âˆ’ [(Î± + Î± âˆ— ) cos Ï† + (Î² + Î² âˆ— ) sin Ï†] sin Î¸ cos Î¸ Ã— Re kâˆ— Î¼âˆ— 1 + kâˆ— 1 (Î± sin Ï† âˆ’ Î² cos Ï†)(Î± âˆ— sin Ï† âˆ’ Î² âˆ— cos Ï†) sin2 Î¸ Re âˆ— Ï‰ Î¼3 Î¾âˆ— Î¼âˆ— 1 âˆ’ (Î±Î² âˆ— + Î± âˆ— Î²) cos Î¸ Re Î¾âˆ— Î¼âˆ— 1 , (35) + sin Î¸ Re (Î± âˆ— sin Ï† + Î² âˆ— cos Ï†) and the scalars Î± and Î² are defined as in Eqs. (25). Ë† Ë† For planewave propagation along the racemic axis (i.e., k = z), only one independent wavenumber, namely kSMCRC = âˆ’kSMCRC = kSMCRC = âˆ’kSMCRC = Ï‰ SPIE Reviews 018003-12 (1) (2) (3) (4) 1 Î¼1 + Î¾ 2, (36) Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . emerges from Eq. (5). The corresponding NPV parameter WSMCRC simplifies as âŽ¤ âŽ¡ âˆ— 2 2 1 Î¼1 + Î¾ Î± âŽ¥ âŽ¢ WSMCRC = + 1 Re âŽ£ âŽ¦ Î² Î¼âˆ— 1 âˆ’ 2Re Î± Î² Re Î¾âˆ— Î¼âˆ— 1 âŽ¡ WSMCRC = Î± Î² Re 1 Î¼1 + Î¾2 âŽ¤ âŽ¥ âŽ¦ for k = kSMCRC , (1),(3) (37) âŽ¢ + 1 Re âŽ£ Î± Î² Î¾âˆ— Î¼âˆ— 1 2 1 Î¼1 + Î¾ âˆ— Î¼âˆ— 1 Re 1 Î¼1 + 2Re Re + Î¾2 for k = kSMCRC . (2),(4) (38) Numerical studies indicate that NPV arises as long as that the magnitude of the magnetoelectric constitutive parameter Î¾ is sufficiently large compared with the magnitudes of dielectric and magnetic constitutive parameters [26]. In addition, the directions of NPV propagation are influenced little by |Î¾ |. Furthermore, the incorporation of dielectric and magnetic constitutive parameters with negative-real parts enhances the propensity for NPV propagation. 2.5 Counterposition, Negative Phase Velocity, and Negative Refraction While NPV may be a useful indicator of the propensity for negative refraction by certain homogeneous materials, NPV can arise in the absence of negative refraction (and vice versa) in certain anisotropic [89] and bianisotropic [90] materials and metamaterials. Furthermore, from a practical point of view, the direction of energy flow, as provided by the time-averaged Poynting vector, may be more pertinent than the direction of the wavevector. Therefore, in the context of NPV and negative refraction, the phenomenon of counterposition should be considered too. This arises at a planar interface when the refraction wavevector and its associated time-averaged Poynting vector are oriented on opposite sides of the normal to the interface, as has been described for certain crystals [91,92]. In order to explore the relationships between counterposition, NPV and negative refraction, let us focus on the Lorentz-reciprocal [88] bianisotropic materialâ€”known as a pseudochiral omega material [93]â€”described by the constitutive dyadics [94] âŽ« Ë†Ë† Ë†Ë† Ë†Ë† âŽª = x xx + y yy + z zz âŽª âŽª âŽª âŽª âŽ¬ Ë†Ë† Î¾ = âˆ’iÎ¾ zy . (39) âŽª Ë†Ë† Î¶ = iÎ¾ yz âŽª âŽª âŽª âŽª âŽ Ë†Ë† Ë†Ë† Ë†Ë† Î¼ = Î¼x xx + Î¼y yy + Î¼z zz These particular constitutive dyadics are used to describe a metamaterial assembled from layers of split-ring resonators [98], this being a commonplace configuration for metamaterials [99,100]. As well as NPV, such magnetoelectric metamaterials may support other exotic electromagnetic phenomenons, for example, longitudinal polarization [101]. Suppose that a metamaterial described by Eqs. (39) fills the half-space z > 0, while the half-space z < 0 is vacuous. The wave vectors of the incident, the reflected, and the refracted plane waves lie wholly in the xz plane. The wavevectors for the two refracted plane waves that exist in the half-space z > 0 may be expressed as Ë† Ë† k(j ) = Îº x + kzj z, SPIE Reviews (j = 1, 2), (40) Vol. 1, 2010 018003-13 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . 0.05 Re kz / k0 0.00 âˆ’0.05 âˆ’0.10 0.0 tanâˆ’1 (k/Re kz) 50 0 âˆ’50 0.0 0.2 0.4 0.6 0.8 1.0 k / k0 (a) k / k0 (b) Fig. 8 (a) Real part of kzj / k 0 and (b) the angle (in degrees) between the real part of k(j ) and the positive z axis, both plotted against Îº/ k 0 . The solid curves correspond to the plane wave labeled j = 1, and the dashed curves to the plane wave labeled j = 2. Note that Im(kzj ) > 0 for all Îº/ k 0 âˆˆ [0, 1), for both values of j. See Sec. 2.5 for other details. where the real-valued Îº = k0 sin Î¸ âˆˆ [0, k0 ) , with the free-space wavenumber k0 = Ï‰ from Eq. (5) as follows: âˆš 0 Î¼0 . (41) The wavevector components kzj are delivered âŽ« âŽª âŽª âŽª âŽª âŽª âŽ¬ Îº2 âˆ’ 2 k0 âŽª âŽª âŽª âŽª âŽª âŽ . (42) kz1 = k0 Î¼x kz2 = k0 x z Îº2 âˆ’ 2 Î¼z k0 âˆ’ Î¾2 z Î¼y Herein, the square roots must be evaluated such that both refracted plane waves transport energy away from the interface z = 0 in the half-space z > 0. Since kzj âˆˆ C in general, the refracted plane waves may be nonuniform. The time-averaged Poynting vector corresponding to the plane wave labeled as j is written as Pj . Confusingly, the term negative refraction has been used to mean different things. The sense of refraction is determined solely by the relative orientations of the real parts of the refraction and incidence wavevectors, in keeping with Snelâ€™s law, which emanates from the principle of conservation of linear momentum. Thus, negative refraction arises whenever the real part of kz1 (or kz2 ) is negative. In contrast, negative refraction was also set up [89] as the negative â€œrefraction of the energy flux density,â€ but it amounts to a negative-deflection phenomenon that can occur whether refraction is positive or negative and is easily appreciated as such when the incident plane wave is replaced by a beam (of finite width). Similar comments apply to certain later works too [95â€“97]. In order to illustrate the distinctions between counterposition, NPV, and negative refraction, let us investigate a specific example in which the constitutive parameters for the bianisotropic material occupying the half-space z > 0 are: x = 0.1 + 0.03i, y = 0.14 + 0.02i, z = 0.13 + 0.07i; Î¼x = âˆ’0.2 + 0.2i, Î¼y = âˆ’0.22 + 0.03i, Î¼z = âˆ’0.27 + 0.6i; and Î¾ = 0.21 + 0.05i. This is a dissipative material. The real part of kzj /k0 , (j = 1, 2), is plotted as a function of (Îº/k0 ) âˆˆ [0, 1) in Fig. 8. Also presented in Fig. 8 are plots of the angle between the real part of k(j ) , (j = 1, 2), and the positive z axis. We see that the refracted plane wave labeled 1 is positively refracted for 0 < (Îº/k0 ) < 0.4 but negatively refracted for 0.4 < (Îº/k0 ) < 1; also, the refracted plane wave labeled 2 is negatively refracted for 0 < (Îº/k0 ) < 0.29 but positively refracted for 0.29 < (Îº/k0 ) < 1. SPIE Reviews 018003-14 Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . 60 Ë† tanâˆ’1 (P . x / P . Ë† z) 0.2 0.4 0.6 0.8 1.0 â€” â€” 0.5 Ë† P.x / P â€” â€” â€” 40 20 0 âˆ’20 âˆ’40 0.0 0.2 0.4 0.6 0.8 1.0 0.0 âˆ’0.5 0.0 k / k0 â€” â€” (a) k / k0 (b) Fig. 9 (a) The x component of the normalized time-averaged Poynting vector and (b) the angle (in degrees) between the time-averaged Poynting vector and the positive z axis, both plotted against Îº/ k 0 . The solid curves correspond to the plane wave labeled j = 1, and the dashed curves to Ë† the plane wave labeled j = 2. Note that z â€¢ P > 0 for all Îº/ k 0 âˆˆ [0, 1), for both plane waves. See Sec. 2.5 for other details. 0.8 0.6 0.4 0.2 0.0 âˆ’0.2 âˆ’0.4 0.0 Re k . P / ( k0 P ) â€” â€” â€” k / k0 Fig. 10 The quantity Re (k(j ) ) â€¢ Pj /(k 0 |Pj |) plotted against (Îº/ k 0 ) âˆˆ [0, 1). The solid curve corresponds to the plane wave labeled j = 1, and the dashed curve to the plane wave labeled j = 2. See Sec. 2.5 for other details. Since the imaginary parts of both kz1 and kz2 are positive, both refracted plane waves attenuate as z â†’ âˆž. In Fig. 9, the normalized x component of the time-averaged Poynting vectors for both refracted plane waves are plotted against (Îº/k0 ). Also plotted is the angle between Pj and the positive z axis, for both refracted plane waves. The x component of P1 is negative for all (Îº/k0 ) âˆˆ [0, 1), but the x component of P2 is negative only for (Îº/k0 ) âˆˆ [0, 0.06). That is, P1 always subtends a negative angle to the positive z axis while the sign of the angle that P2 subtends depends on Îº. The z components of Pj for both refracted plane waves are positive for all (Îº/k0 ) âˆˆ [0, 1), as is required by the choice of square roots in Eq. (42). When the inequality x Re(kzj )Ë† â€¢ Pj < 0 (43) is satisfied, counterposition occurs [92]. From Figs. 8 and 9, it may be inferred that counterposition occurs for the refracted plane wave labeled 1 when 0 < (Îº/k0 ) < 0.4. Hence, the Îº-range for positive refraction is the same as that for counterposition for the planewave labeled 1. This contrasts with the situation for the plane wave labeled 2 where counterposition arises only for 0.06 < (Îº/k0 ) < 0.29. The sign of the phase velocity for the plane wave labeled j is determined the quantity Re (k(j ) ) â€¢ Pj , which is plotted against (Îº/k0 ) âˆˆ [0, 1) in Fig. 10. The refracted plane wave labeled 1 has NPV for 0.18 < (Îº/k0 ) < 1, whereas NPV is exhibited by the refracted plane wave labeled 2 for 0 < (Îº/k0 ) < 0.08. Notice that the Îºâ€“ranges for NPV and negative refraction do not coincide. Take, for example, Îº = 0.2k0 : (i) The angle between Re (k(1) ) and the +z axis is 79 deg and the angle between P1 and the +z axis is âˆ’15 deg. Thus, here the plane wave is SPIE Reviews 018003-15 Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . Table 1 Values of Îº for which negative/positive refraction, counterposition, and negative/positive/orthogonal phase velocity occur for the plane wave labeled 1. The right-most column shows the directions in the half-space z > 0 of Re(k(1) ) (thick dashed arrows) and P1 (thick solid arrows) for representative values of Îº; also shown are the directions of the wavevectors for the incident and reï¬‚ected plane waves in the half-space z < 0 (thin solid arrows). (Îº/ k 0 ) âˆˆ Refraction Counter-position Phase velocity P1 , Re(k(1) ) (0, 0.18) +ve yes +ve {0.18} +ve yes orthogonal (0.18, 0.4) +ve yes âˆ’ve (0.4, 1) âˆ’ve no âˆ’ve positively refracted but it has NPV. (ii) The angle between Re (k(2) ) and the +z axis is âˆ’87 deg and the angle between P2 and the +z axis is 50 deg. This plane wave is negatively refracted despite having positive phase velocity. Exceptionally, the phase velocity can be neither positive nor negative. At Îº = 0.18k0 , the phase velocity vector and the time-averaged Poynting vector are orthogonal for the plane wave labeled 1. Orthogonal phase velocity occurs for the plane wave labeled 2 at Îº = 0.08k0 . The foregoing results are summarized in Tables 1 and 2 for the plane waves labeled 1 and 2, respectively. Included in these tables are illustrations of the directions of Re (k(j ) ) and Pj (j = 1, 2), for representative values of Îº. This numerical example illustrates the complexity that can arise at the planar boundary of a chiral metamaterialâ€”indeed, the independence of negative refraction and NPV can even arise for isotropic dielectric materials if nonuniform plane waves are taken into consideration [90]. SPIE Reviews 018003-16 Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . Table 2 As Table 1 but for the plane wave labeled 2. (Îº/ k 0 ) âˆˆ Refraction Counter-position Phase velocity P2 , Re(k(2) ) (0, 0.06) âˆ’ve no âˆ’ve (0.06, 0.08) âˆ’ve yes âˆ’ve {0.08} âˆ’ve yes orthogonal (0.08, 0.29) âˆ’ve yes +ve (0.29, 1) +ve no +ve SPIE Reviews 018003-17 Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . 3 Structurally Chiral Materials 3.1 Preliminaries In contrast to the materials considered in Sec. 2, structurally chiral materials owe their chirality to the handedness of their morphology at macroscopic length scales (i.e., at length scales comparable to the wavelength). A very general class of structurally chiral materials is represented by helicoidal bianisotropic materials (HBMs). These include chiral nematic and chiral smectic liquid crystals as well as sculptured thin films. The nonhomogeneity of HBMsâ€”which gives rise to their chiralityâ€”is spatially continuous at macroscopic length scales. Another technologically important type of structurally chiral material is represented by ambichiral materials. These are piecewise homogeneous in a certain direction [32]. The propensity of both HBMs and ambichiral materials to support negative refraction is reviewed in the following sections. 3.2 Helicoidal Bianisotropic Materials The frequency-domain constitutive relations [102] D(r) = H BM (z) â€¢ E(r) + Î¾H BM (z) â€¢ H(r) B(r) = Î¶H BM (z) â€¢ E(r) + Î¼H BM (z) â€¢ H(r) (44) describe a HBM with the z axis being the helicoidal axis. The four 3Ã—3 nonhomogeneous constitutive dyadics herein have the general form âŽž âŽ› Î²11 (z) Î²12 (z) Î²13 (z) âŽŸ âŽœ (45) Î²H BM (z) = âŽœ Î²21 (z) Î²22 (z) Î²23 (z) âŽŸ , (Î² = , Î¾, Î¶, Î¼), âŽ âŽ Î²31 (z) Î²32 (z) Î²33 (z) and may be expressed as Î²H BM (z) = S(z) â€¢ Î²H BM (0) â€¢ Sâˆ’1 (z), (Î² = , Î¾, Î¶, Î¼). âŽž (47) (46) The helicoidal architecture is specified by the rotation dyadic âŽ› Ï€z Ï€z cos âˆ’h sin âŽœ âŽœ Ï€z S(z) = âŽœ h sin Ï€ z cos âŽœ âŽ 0 0 âŽŸ âŽŸ âŽŸ 0âŽŸ, âŽ 1 with being the half-period. The HBM is structurally right-handed if h = 1, left-handed if h = âˆ’1, and structurally achiral if h = 0. A host of structurally chiral materials are encompassed by the constitutive Eqs. (44). The chirality may be purely dielectric, in which case Î¾H BM = Î¶H BM = 0 and Î¼H BM = Î¼0 I. This subcategory includes chiral nematic liquid crystals (wherein H BM has a uniaxial form), chiral smectic liquid crystals (wherein H BM has a biaxial form) [30,31]; and their solid-state counterparts called chiral sculptured thin films [33]. Illustrations of organic and inorganic chiral sculptured thin films, both fabricated by vapor deposition techniques, are provided in Fig. 11. The chirality may also be purely magnetic, in which case Î¾H BM = Î¶H BM = 0 and H BM = 0 I. Fully bianisotropic chirality may be achieved through infiltrating a chiral sculptured thin film with an isotropic chiral fluid [104,105]. Most notably, HBMs can discriminate between left- and right-circularly polarized light. Let us consider a plane wave normally incident on a slab of an HBM that has its helicoidal axis SPIE Reviews 018003-18 Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . Fig. 11 Scanning electron microscope images of chiral sculptured thin ï¬lms made from silicon oxide (top, Courtesy of Mark W. Horn, Pennsylvania State University) and parylene [103] (bottom). aligned with the direction of slab thickness. Within a certain wavelength regime, the incident light may be almost entirely reflected if the structural handedness of the HBM coincides with the handedness of the incident light. Conversely, if the two handednesses are opposite then the incident light will undergo almost no reflection. This circular Bragg phenomenon underpins many actual and potential technological applications of HBMs [33]. The propagation of plane waves in HBMs has been comprehensively analyzed [102,106]. Combining the constitutive Eqs. (44) with the source-free Maxwell curl postulates yields the system of partial differential equations âˆ‡ Ã— E(r) = iÏ‰ [Î¶H BM (z) â€¢ E(r) + Î¼H BM (z) â€¢ H(r)] âˆ‡ Ã— H(r) = âˆ’iÏ‰ [ H BM (z) â€¢ E(r) + Î¾H BM (z) â€¢ H(r)] (48) Upon implementing the Oseen transformation [109] E (r) = Sâˆ’1 (z) â€¢ E(r) H (r) = Sâˆ’1 (z) â€¢ H(r) SPIE Reviews 018003-19 (49) Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . and introducing the planewave representations E (r) = E0 (z) exp (iÎºH BM x) H (r) = H0 (z) exp (iÎºH BM x) , (50) wherein ÎºH BM may be interpreted as a wavenumber in the xy plane, Eqs. (48) generally reduce to the 4Ã—4 matrix differential equation âˆ‚ F (z) = M (z) â€¢ F0 (z). âˆ‚z 0 Herein, the column 4-vector âŽ¡ âŽ¢ âŽ¥ âŽ¢ y â€¢ E (z) âŽ¥ 0 âŽ¢Ë† âŽ¥ F0 (z) = âŽ¢ âŽ¥, âŽ¢ x â€¢ H (z) âŽ¥ Ë† 0 âŽ£ âŽ¦ Ë† y â€¢ H0 (z) and the 4Ã—4 matrix function M (z) may be formally expressed as M (z) = A + ÎºH BM C1,1 exp 2 + ÎºH BM C2,2 exp (51) Ë† x â€¢ E0 (z) âŽ¤ (52) iÏ€ z + C1,âˆ’1 exp âˆ’ iÏ€ z i2Ï€ z i2Ï€ z + C2,0 + C2,âˆ’2 exp âˆ’ (53) with the 4 Ã— 4 matrixes A , C1,Â±1 , C2,0 , and C2,Â±2 being independent of z and ÎºH BM but not of the half-period and the handedness parameter h. Explicit representations of M (z, Ï‰) are straightforwardly derived but cumbersome; the reader is referred elsewhere for further details [33]. In the case of axial propagation (i.e., ÎºH BM = 0), the solution to Eq. (51) is conveniently expressed in closed form as [102] F0 (z) = exp(iA z)F0 (0). (54) The nonaxial propagation case (i.e., ÎºH BM = 0) is considerably more complicated to handle. However, Eq. (53) can be exploited to derive a solution to Eq. (51) in terms of a power series in z [106]. As an alternative, a piecewise uniform approximation may also be implemented [107,108]. The propensity of HBMs to exhibit characteristics related to negative refraction has been explored for the particular cases of chiral ferronematic materials (which are characterized by the constitutive relations in Eq. (44) with H BM and Î¼H BM having uniaxial forms, and the magnetoelectric dyadics Î¾H BM and Î¶H BM being null valued) [27] and chiral ferrosmectic materials (which are characterized by the constitutive Eqs. (44) with H BM and Î¼H BM having biaxial forms, and the magnetoelectric dyadics Î¾H BM and Î¶H BM being null valued) [28]. In both instances, it was observed that the structural handedness of the materials is effectively reversed when the real parts of the permittivity and permeability parameters are changed from positive to negative. That is, a structurally right/left-handed HBM with negative real permittivity and permeability parameters exhibits the circular Bragg phenomenon as though it were a structurally left/right-handed HBM with positive real permittivity and permeability parameters. Furthermore, when the real parts of the permittivity and permeability parameters are changed from positive to negative, the reflection and transmission coefficients undergo a phase reversal that can result SPIE Reviews 018003-20 Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . Fig. 12 The ambichiral metamaterial of Plum et al. [117]. The structure is based on layers of metallic rosettes. The rosettes in consecutive layers have a relative twist of 15 deg. (Reprinted with permission from Ref. 117. Copyright 2009 by the American Physical Society.) in negative Goosâ€“HÂ¨ nchen shifts [28]. Such negative Goosâ€“HÂ¨ nchen shifts are a characteristic a a of materials that support NPV [110â€“113]. 3.3 Ambichirality Imagine a uniaxial crystalline sheet whose distinguished axis is oriented normal to the sheetâ€™s thickness direction. Now consider stack of such sheets with the angle between the distinguished axes of each pair of neighbouring sheets being Ï€/q, q = 2, 3, . . . . For q > 2 this stack represents an ambichiral material, as originally conceived by Reusch [32] and later analyzed by Joly and Billard [114]. As is true for HBMs (which may be viewed as the limiting case q â†’ âˆž), ambichiral materials can exhibit different Bragg resonances for different circular polarization states.â€ However, if the dielectric and magnetic dyadics of the underlying constituent materials are indefinite, the corresponding ambichiral material loses its ability to discriminate between different circular polarization states, provided that the number of constituent sheets is sufficiently large. This propertyâ€”which arises because two of the four planewave components in each sheet are of the NPV type and two are of the positive-phase-velocity typeâ€”enables such an ambichiral material to function as a polarization-universal rejection filter [116]. The ambichiral architecture essentially underpins a recent report by Plum et al. [117] of a negatively refracting metamaterial, based on a stack of sheets each containing metallic rosettes with every sheet rotated about the normal axis with respect to the previous sheet in the stack by an angle less that 90 deg. An illustration is provided in Fig. 12. A similarly stacked chiral metamaterial that supports negative refraction, with a cross-wire microstructure, has been described by Zhou et al. [118]. 4 Closing Remarks The interaction of light with chiral metamaterials presents promising opportunities. In this review we have highlighted the propensity of these metamaterials to support negative refraction and closely related phenomenons. However, these opportunities come at a price: there are also formidable challenges, both experimental and theoretical, associated with chiral metamaterials. As we highlight in Sec. 2.5, the characterization of the complex behavior exhibited by these metamaterials requires careful treatment. In particular, optical properties cannot be characterized â€ The q = 2 caseâ€”which corresponds to an equichiral materialâ€”is of little technological interest as such materials exhibit the same Bragg resonances for both circular polarization states [115]. SPIE Reviews 018003-21 Vol. 1, 2010 Mackay and Lakhtakia: Negatively refracting chiral metamaterials . . . Fig. 13 Two of the eight sculptures from the permanent installation The Matter of Time by Richard Serra at the Guggenheim Museum Bilbao. The sculpture on the left may remind the reader of a Swiss roll, the one on the right of a double split-ring resonator, both structures commonplace in the literature on negatively refracting metamaterials. Were the metal sheets in both sculptures strictly vertical, both would be achiral. by a simple scalar refractive index that refers only to one mode of propagation, along one direction only. Instead, multiple wavevectors, which may be directionally dependent, need to be considered. The comprehensive characterization of optical properties may involve significant distinctions still being made between counterposition, NPV, and negative refraction. A perusal of ongoing experimental research on optical (frequency 500 THz) metamaterials shows that standard micro- and nano-fabrication techniques are being used to make them [12â€“15,100,119â€“122]. Metamaterials for operation at frequencies exceeding 500 THz would have to be engineered on the nanoscale [15,119]. Remarkable optical effects can be expected from nanoengineered metamaterials, as nanotechnology for optics is a play of phase, length, and time [123]. As quantum-confinement effects will also emerge at higher frequencies [124], a strict scaling down of classical electromagnetics [125] may not suffice for designing both metamaterials and metamaterial-based devices. The associated difficulties are likely to be accentuated for asymmetric morphology at the nanoscale and, thus, for chiral metamaterials. To compensate, we must note that nanofabrication methods [126â€“128] are suited well to produce assemblies of different kinds of electrically small cells for multifunctional performance at the macroscopic scale. While metamaterials (chiral or otherwise) have much to offer, after the past nine years or more of intensive research there still remains a wide gulf between the research frontier and practical applications [129]. One major issue to be tackled is the dissipation of electromagnetic energy in a material of reasonable thickness. Either pre-amplification or the incorporation of gain materials appears necessary, though we must note that the energy budget may then turn out to be economically impractical. Another major issue is the rapid variation of constitutive parameters with frequency in the frequency regimes of interest. This large dispersion could significantly distort pulse-modulated waves. Ingenuity and perseveranceâ€”perhaps, along with serendipityâ€”are needed to find economically viable metamaterials that refract negatively.

SPIE Reviews – SPIE

**Published: ** Jan 1, 2010

Loading...

You can share this free article with as many people as you like with the url below! We hope you enjoy this feature!

Read and print from thousands of top scholarly journals.

System error. Please try again!

Already have an account? Log in

Bookmark this article. You can see your Bookmarks on your DeepDyve Library.

To save an article, **log in** first, or **sign up** for a DeepDyve account if you don’t already have one.

Copy and paste the desired citation format or use the link below to download a file formatted for EndNote

Access the full text.

Sign up today, get DeepDyve free for 14 days.

All DeepDyve websites use cookies to improve your online experience. They were placed on your computer when you launched this website. You can change your cookie settings through your browser.